Non-Destructive Inspection of High Temperature Piping Combining Ultrasound and Eddy Current Testing

This paper presents an automated Non-Destructive Testing (NDT) system for the in-service inspection of orbital welds on tubular components operating at temperatures as high as 200 °C. The combination of two different NDT methods and respective inspection systems is here proposed to cover the detection of all potential defective weld conditions. The proposed NDT system combines ultrasounds and Eddy current techniques with dedicated approaches for dealing with high temperature conditions. Phased array ultrasound was employed, searching for volumetric defects within the weld bead volume while Eddy currents were used to look for surface and sub-surface cracks. The results from the phased array ultrasound results showed the effectiveness of the cooling mechanisms and that temperature effects on sound attenuation can be easily compensated for up to 200 °C. The Eddy current results showed almost no influence when temperatures were raised up to 300 °C.


Introduction
Non-Destructive Evaluation (NDE) is continuously improving and changing. New techniques and challenges arising from new materials and manufacturing processes are continuously pushing Non-Destructive Testing (NDT) forward [1,2]. One good example concerns in-service high-temperature component inspection, whose industrial relevancy is easily sustained [3]. Components such as steam transportation pipelines must withstand high temperatures above 300 • C, requiring adapted in-service inspection and condition monitoring methods. There are several solutions for pipe inspection [4], but few application examples can be found for when high temperature conditions apply and where customized equipment is required [5][6][7][8].
The literature reports high-temperature NDT applications including permanent inspections of hot wire [5] and in-situ monitoring using Eddy currents [9] and ultrasound [10,11]. In these works, equipment was developed and/or adapted to answer the specific requirements of the end application, and could not be adapted to other uses.
High-Temperature Ultrasonic Testing (HTUT) has been continuously developed, driven by substantial industrial interest. Ultrasound Testing (UT) allows the inspection of optically opaque materials such as liquid-metal coolants, steam generator piping, and heat exchanger pipes [10]. However, the temperature at which ultrasonic transducers The developed standard block had a tubular geometry with two butt welds. The block base material was a class P235GH steel as specified in EN 10216-2 [25], suitable for high temperature and/or high pressure operating conditions. The standard block butt welds were carried out according to the specification WPS.141.01. These welds are characterized by a root step, applying the TIG method, proceeded by filling using coated electrodes. The manufactured standard block and the corresponding dimensions are presented in Table 1.
After performing ultrasound and X-ray NDT to ensure that no unintentional defects existed in the weld, three artificial defects were manufactured. These three defects-a weld toe notch, a weld root notch, and a weld bevel flat bottom hole-were chosen to represent traditionally found defects according to the paper pulp factory owner, and their characteristics were based on the standard blocks specified in ISO 13588 [26]. The artificially manufactured defects are specified in Table 2. characteristics were based on the standard blocks specified in ISO 13588 [26]. The artificially manufactured defects are specified in Table 2.

Automated Inspection System
To perform inspections on high-temperature components with contact-requiring techniques, it is crucial to use a semi/full automated system. The system was developed to ensure proper ultrasonic/eddy current probe contact and positioning over the weld bead and to maximize the operator's distance from the high-temperature component. The automated inspection system comprised a scanner attached to an orbital guide that was installed in the vicinity of the weld that was to be inspected. The guide included a hinge mechanism to allow for simple and fast installation around the pipe. Different probes could be mounted in the scanner using dedicated holders for ultrasonic and Eddy current probes. Figure 1 shows the scanning system mounted on the standard block. characteristics were based on the standard blocks specified in ISO 13588 [26]. The artificially manufactured defects are specified in Table 2.

Automated Inspection System
To perform inspections on high-temperature components with contact-requiring techniques, it is crucial to use a semi/full automated system. The system was developed to ensure proper ultrasonic/eddy current probe contact and positioning over the weld bead and to maximize the operator's distance from the high-temperature component. The automated inspection system comprised a scanner attached to an orbital guide that was installed in the vicinity of the weld that was to be inspected. The guide included a hinge mechanism to allow for simple and fast installation around the pipe. Different probes could be mounted in the scanner using dedicated holders for ultrasonic and Eddy current probes. Figure 1 shows the scanning system mounted on the standard block.  characteristics were based on the standard blocks specified in ISO 13588 [26]. The artificially manufactured defects are specified in Table 2.

Automated Inspection System
To perform inspections on high-temperature components with contact-requiring techniques, it is crucial to use a semi/full automated system. The system was developed to ensure proper ultrasonic/eddy current probe contact and positioning over the weld bead and to maximize the operator's distance from the high-temperature component. The automated inspection system comprised a scanner attached to an orbital guide that was installed in the vicinity of the weld that was to be inspected. The guide included a hinge mechanism to allow for simple and fast installation around the pipe. Different probes could be mounted in the scanner using dedicated holders for ultrasonic and Eddy current probes. Figure 1 shows the scanning system mounted on the standard block. characteristics were based on the standard blocks specified in ISO 13588 [26]. The artificially manufactured defects are specified in Table 2.

Automated Inspection System
To perform inspections on high-temperature components with contact-requiring techniques, it is crucial to use a semi/full automated system. The system was developed to ensure proper ultrasonic/eddy current probe contact and positioning over the weld bead and to maximize the operator's distance from the high-temperature component. The automated inspection system comprised a scanner attached to an orbital guide that was installed in the vicinity of the weld that was to be inspected. The guide included a hinge mechanism to allow for simple and fast installation around the pipe. Different probes could be mounted in the scanner using dedicated holders for ultrasonic and Eddy current probes. Figure 1 shows the scanning system mounted on the standard block. characteristics were based on the standard blocks specified in ISO 13588 [26]. The artificially manufactured defects are specified in Table 2.

Automated Inspection System
To perform inspections on high-temperature components with contact-requiring techniques, it is crucial to use a semi/full automated system. The system was developed to ensure proper ultrasonic/eddy current probe contact and positioning over the weld bead and to maximize the operator's distance from the high-temperature component. The automated inspection system comprised a scanner attached to an orbital guide that was installed in the vicinity of the weld that was to be inspected. The guide included a hinge mechanism to allow for simple and fast installation around the pipe. Different probes could be mounted in the scanner using dedicated holders for ultrasonic and Eddy current probes. Figure 1 shows the scanning system mounted on the standard block.

Automated Inspection System
To perform inspections on high-temperature components with contact-requiring techniques, it is crucial to use a semi/full automated system. The system was developed to ensure proper ultrasonic/Eddy current probe contact and positioning over the weld bead and to maximize the operator's distance from the high-temperature component. The automated inspection system comprised a scanner attached to an orbital guide that was installed in the vicinity of the weld that was to be inspected. The guide included a hinge mechanism to allow for simple and fast installation around the pipe. Different probes could be mounted in the scanner using dedicated holders for ultrasonic and Eddy current probes. Figure 1 shows the scanning system mounted on the standard block. The inspection system was composed of five main features: • Orbital guide around the pipe, enabling the scanner's movement-element 1; • Quick tightening joint, to attach the scanner to the orbital guide-element 2; • Air-cooled housing, to shelter the DC motors-element 3; • Water-cooled base plate, where the DC motors were fixed-element 4; • Probe holder-element 5.
The orbital guide around the pipe ( Figure 1, element 1) consisted of two halves, with a swivel joint at one end and a fastening system with only one screw at the other end. The guide supports to the tube were adjustable, allowing the same guide to be used in different tube diameters within a range of 30 mm. A quick tightening joint- Figure 1, element 2allowed for engagement of the scanner in the guide by manually tightening a screw.
The driving system gear engaged the orbital guide (with toothed sides), ensuring power transmission and avoiding landslides due to the scanner's own weight. The body of the scanner consisted of two housings- Figure 1, element 3-each incorporating a DC motor coupled to a toothed drive wheel. This system was cooled by compressed air inside the housing. The DC motors base plate was water-cooled as in Figure 1, element 4. The two brushed DC motors were a A-max 32 model from Maxon ® as well as the positioning controller EPOS2 24/5.
The pipe temperature was monitored during the high-temperature inspections with a thermographic camera Fluke Ti400 with an emissivity index of 0.95, as depicted in Figure 2. The inspection system was composed of five main features:

•
Orbital guide around the pipe, enabling the scanner's movement-element 1; • Quick tightening joint, to attach the scanner to the orbital guide-element 2; • Air-cooled housing, to shelter the DC motors-element 3; • Water-cooled base plate, where the DC motors were fixed-element 4; • Probe holder-element 5.
The orbital guide around the pipe ( Figure 1, element 1) consisted of two halves, with a swivel joint at one end and a fastening system with only one screw at the other end. The guide supports to the tube were adjustable, allowing the same guide to be used in different tube diameters within a range of 30 mm. A quick tightening joint- Figure 1, element 2-allowed for engagement of the scanner in the guide by manually tightening a screw.
The driving system gear engaged the orbital guide (with toothed sides), ensuring power transmission and avoiding landslides due to the scanner's own weight. The body of the scanner consisted of two housings- Figure 1, element 3-each incorporating a DC motor coupled to a toothed drive wheel. This system was cooled by compressed air inside the housing. The DC motors base plate was water-cooled as in Figure 1, element 4. The two brushed DC motors were a A-max 32 model from Maxon ® as well as the positioning controller EPOS2 24/5.
The pipe temperature was monitored during the high-temperature inspections with a thermographic camera Fluke Ti400 with an emissivity index of 0.95, as depicted in Figure 2.

Heating and Temperature Control
To perform the laboratorial experimental tests with the standard block at high temperatures, a heating system was designed and manufactured. Heat was generated through eight 1000 W electrical resistances driven by 4 rheostats (each rheostat controlled 2 electrical resistances), inserted inside the standard block as shown in Figure 3.

Heating and Temperature Control
To perform the laboratorial experimental tests with the standard block at high temperatures, a heating system was designed and manufactured. Heat was generated through eight 1000 W electrical resistances driven by 4 rheostats (each rheostat controlled 2 electrical resistances), inserted inside the standard block as shown in Figure 3. Heat regulation was performed by adjusting the rheostats and controlling the electrical resistances, dissipating the power. To conduct the tests, small increments of electrical power were made to achieve a total of 8 temperature steps from room temperature to 200 °C. A 2 h interval was maintained between increments so that the standard block temperature could stabilize before the experimental tests. Temperature control and recording was carried out with a thermometer (Tempil IRT-16, temperature range −60 °C to 625 °C).

Probe and Wedge Concept
It was considered that temperature increases have two direct consequences on ultrasound inspections: increased attenuation and increased propagation speed. It is possible to reduce the attenuation of sound waves by using lower-frequency probes; however, it must be noted that this also lowers the sensitivity. Concerning propagation speed increases, these can be easily measured and corrected in the used instrumentation.

Heating and Temperature Control
To perform the laboratorial experimental tests with the standard block at high temperatures, a heating system was designed and manufactured. Heat was generated through eight 1000 W electrical resistances driven by 4 rheostats (each rheostat controlled 2 electrical resistances), inserted inside the standard block as shown in Figure 3. Heat regulation was performed by adjusting the rheostats and controlling the electrical resistances, dissipating the power. To conduct the tests, small increments of electrical power were made to achieve a total of 8 temperature steps from room temperature to 200 °C. A 2 h interval was maintained between increments so that the standard block temperature could stabilize before the experimental tests. Temperature control and recording was carried out with a thermometer (Tempil IRT-16, temperature range −60 °C to 625 °C).

Probe and Wedge Concept
It was considered that temperature increases have two direct consequences on ultrasound inspections: increased attenuation and increased propagation speed. It is possible to reduce the attenuation of sound waves by using lower-frequency probes; however, it must be noted that this also lowers the sensitivity. Concerning propagation speed increases, these can be easily measured and corrected in the used instrumentation. Heat regulation was performed by adjusting the rheostats and controlling the electrical resistances, dissipating the power. To conduct the tests, small increments of electrical power were made to achieve a total of 8 temperature steps from room temperature to 200 • C. A 2 h interval was maintained between increments so that the standard block temperature could stabilize before the experimental tests. Temperature control and recording was carried out with a thermometer (Tempil IRT-16, temperature range −60 • C to 625 • C).

Probe and Wedge Concept
It was considered that temperature increases have two direct consequences on ultrasound inspections: increased attenuation and increased propagation speed. It is possible to reduce the attenuation of sound waves by using lower-frequency probes; however, it must be noted that this also lowers the sensitivity. Concerning propagation speed increases, these can be easily measured and corrected in the used instrumentation. The real problem occurs when the test piece presents a temperature gradient along the propagation direction of the sound beam, as in most practical situations. This temperature gradient affects the sound wave velocity-thus causing the sound beam deviation. Figure 4 depicts a phased array shim with a temperature gradient; the orange line represents the beam direction in normal conditions while the green line is the deviation suffered due to the temperature gradient. This deviation is relatively small, although this effect is amplified as sound waves propagate through the piece.
propagation direction of the sound beam, as in most practical situations. This temperature gradient affects the sound wave velocity-thus causing the sound beam deviation. Figure  4 depicts a phased array shim with a temperature gradient; the orange line represents the beam direction in normal conditions while the green line is the deviation suffered due to the temperature gradient. This deviation is relatively small, although this effect is amplified as sound waves propagate through the piece. Distinct phased array probes were studied with the simulation software EXTEND CIVA 2017, looking for the best options. A 20-element linear phased array probe IMASONIC ® 12051 operating at 3.25 MHz was selected, providing enhanced flaw responses (in terms of signal amplitude) and signal to noise ratios. The probe specifications are presented in Table 3. The selected phased array probe had a maximum operating temperature of 60 °C; therefore, a water-cooled housing was required to ensure that the wedge top and the probe remained cool during operation. Figure 5 presents the adopted wedge and probe configuration.  Distinct phased array probes were studied with the simulation software EXTEND CIVA 2017, looking for the best options. A 20-element linear phased array probe IMASONIC ® 12051 operating at 3.25 MHz was selected, providing enhanced flaw responses (in terms of signal amplitude) and signal to noise ratios. The probe specifications are presented in Table 3. The selected phased array probe had a maximum operating temperature of 60 • C; therefore, a water-cooled housing was required to ensure that the wedge top and the probe remained cool during operation. Figure 5 presents the adopted wedge and probe configuration. gradient affects the sound wave velocity-thus causing the sound beam deviation. Figure  4 depicts a phased array shim with a temperature gradient; the orange line represents the beam direction in normal conditions while the green line is the deviation suffered due to the temperature gradient. This deviation is relatively small, although this effect is amplified as sound waves propagate through the piece. Distinct phased array probes were studied with the simulation software EXTEND CIVA 2017, looking for the best options. A 20-element linear phased array probe IMASONIC ® 12051 operating at 3.25 MHz was selected, providing enhanced flaw responses (in terms of signal amplitude) and signal to noise ratios. The probe specifications are presented in Table 3. The selected phased array probe had a maximum operating temperature of 60 °C; therefore, a water-cooled housing was required to ensure that the wedge top and the probe remained cool during operation. Figure 5 presents the adopted wedge and probe configuration.  Additionally, wedges made of heat-resistant materials were tried in order to cope with the high temperatures. A wedge produced in Duratron ® PBI (Polybenzimidazole) was produced to withstand temperatures of up to 200 • C. This polymer material, developed by Quadrant Plastics, has announced temperature services at up to 310 • C continuously and up to 500 • C for short periods of time. Another characteristic of this material is its low thermal expansion coefficient and constant material properties up to 400 • C [9].
The wedge material had a longitudinal ultrasound velocity of 2970 m/s and a 25.7 • wedge angle, producing a 60 • central angle in the standard block. An appropriate couplant was necessary to ensure good and constant ultrasound transmission between the probe and the piece. The couplant must have high wettability, corrosion resistance and proper viscosity and removal properties. Since traditional water and gel-based couplants cannot be used at high temperatures, a vegetable oil was used instead, after verifying that it is non-flammable at the involved temperatures nor produces irritant or harmful smokes for the operator.

Focal Laws
For each produced artificial defect, a dedicated focal law was defined to enhance detectability in each zone of the weld. These focal laws were defined bearing in mind ISO 17640 [26] and ISO 13588 [27]. A sectorial scan ensures normal wave incidence with a half skip to the bevel and accounts for minor deviations in the weld bevel angle.
A combination of sectorial scanning with electronic scanning was used for the flat bottom hole in the bevel (simulating a lack of fusion). In this case, longitudinal ultrasound waves with half-skips are used to generate the desired angles and to ensure complete coverage of the weld. The notch in the weld toe simulates a crack next to the weld or in the Heat Affected Zone (HAZ), so a half-skip is also needed to obtain the desired coverage. In this case, transversal ultrasound waves were used, with a combination of sectorial and electronic scanning. Simulating cracks in the root, the detection of this notch was made through longitudinal waves in direct mode (no skips), as well as with a combination of electronic and sectorial scanning. Three focal laws were defined-one for each defect type. Version 6.9.25 of the Multi2000 software and MULTIX++ hardware, both from the company M2M, were used for data acquisition and processing. Table 4 presents the parameters of each focal law, as well as the corresponding beam coverage. Table 4. Characteristics and beam coverage representation of each focal law.

Weld bevel flat bottom hole
with the high temperatures. A wedge produced in Duratron PBI (Polybenzimidazole) was produced to withstand temperatures of up to 200 °C. This polymer material, developed by Quadrant Plastics, has announced temperature services at up to 310 °C continuously and up to 500 °C for short periods of time. Another characteristic of this material is its low thermal expansion coefficient and constant material properties up to 400 °C [9].
The wedge material had a longitudinal ultrasound velocity of 2970 m/s and a 25.7° wedge angle, producing a 60° central angle in the standard block. An appropriate couplant was necessary to ensure good and constant ultrasound transmission between the probe and the piece. The couplant must have high wettability, corrosion resistance and proper viscosity and removal properties. Since traditional water and gel-based couplants cannot be used at high temperatures, a vegetable oil was used instead, after verifying that it is non-flammable at the involved temperatures nor produces irritant or harmful smokes for the operator.

Focal Laws
For each produced artificial defect, a dedicated focal law was defined to enhance detectability in each zone of the weld. These focal laws were defined bearing in mind ISO 17640 [26] and ISO 13588 [27]. A sectorial scan ensures normal wave incidence with a half skip to the bevel and accounts for minor deviations in the weld bevel angle.
A combination of sectorial scanning with electronic scanning was used for the flat bottom hole in the bevel (simulating a lack of fusion). In this case, longitudinal ultrasound waves with half-skips are used to generate the desired angles and to ensure complete coverage of the weld. The notch in the weld toe simulates a crack next to the weld or in the Heat Affected Zone (HAZ), so a half-skip is also needed to obtain the desired coverage. In this case, transversal ultrasound waves were used, with a combination of sectorial and electronic scanning. Simulating cracks in the root, the detection of this notch was made through longitudinal waves in direct mode (no skips), as well as with a combination of electronic and sectorial scanning. Three focal laws were defined-one for each defect type. Version 6.9.25 of the Multi2000 software and MULTIX++ hardware, both from the company M2M, were used for data acquisition and processing. Table 4 presents the parameters of each focal law, as well as the corresponding beam coverage. with the high temperatures. A wedge produced in Duratron PBI (Polybenzimidazole) was produced to withstand temperatures of up to 200 °C. This polymer material, developed by Quadrant Plastics, has announced temperature services at up to 310 °C continuously and up to 500 °C for short periods of time. Another characteristic of this material is its low thermal expansion coefficient and constant material properties up to 400 °C [9]. The wedge material had a longitudinal ultrasound velocity of 2970 m/s and a 25.7° wedge angle, producing a 60° central angle in the standard block. An appropriate couplant was necessary to ensure good and constant ultrasound transmission between the probe and the piece. The couplant must have high wettability, corrosion resistance and proper viscosity and removal properties. Since traditional water and gel-based couplants cannot be used at high temperatures, a vegetable oil was used instead, after verifying that it is non-flammable at the involved temperatures nor produces irritant or harmful smokes for the operator.

Focal Laws
For each produced artificial defect, a dedicated focal law was defined to enhance detectability in each zone of the weld. These focal laws were defined bearing in mind ISO 17640 [26] and ISO 13588 [27]. A sectorial scan ensures normal wave incidence with a half skip to the bevel and accounts for minor deviations in the weld bevel angle.
A combination of sectorial scanning with electronic scanning was used for the flat bottom hole in the bevel (simulating a lack of fusion). In this case, longitudinal ultrasound waves with half-skips are used to generate the desired angles and to ensure complete coverage of the weld. The notch in the weld toe simulates a crack next to the weld or in the Heat Affected Zone (HAZ), so a half-skip is also needed to obtain the desired coverage. In this case, transversal ultrasound waves were used, with a combination of sectorial and electronic scanning. Simulating cracks in the root, the detection of this notch was made through longitudinal waves in direct mode (no skips), as well as with a combination of electronic and sectorial scanning. Three focal laws were defined-one for each defect type. Version 6.9.25 of the Multi2000 software and MULTIX++ hardware, both from the company M2M, were used for data acquisition and processing. Table 4 presents the parameters of each focal law, as well as the corresponding beam coverage. was produced to withstand temperatures of up to 200 °C. This polymer material, developed by Quadrant Plastics, has announced temperature services at up to 310 °C continuously and up to 500 °C for short periods of time. Another characteristic of this material is its low thermal expansion coefficient and constant material properties up to 400 °C [9]. The wedge material had a longitudinal ultrasound velocity of 2970 m/s and a 25.7° wedge angle, producing a 60° central angle in the standard block. An appropriate couplant was necessary to ensure good and constant ultrasound transmission between the probe and the piece. The couplant must have high wettability, corrosion resistance and proper viscosity and removal properties. Since traditional water and gel-based couplants cannot be used at high temperatures, a vegetable oil was used instead, after verifying that it is non-flammable at the involved temperatures nor produces irritant or harmful smokes for the operator.

Focal Laws
For each produced artificial defect, a dedicated focal law was defined to enhance detectability in each zone of the weld. These focal laws were defined bearing in mind ISO 17640 [26] and ISO 13588 [27]. A sectorial scan ensures normal wave incidence with a half skip to the bevel and accounts for minor deviations in the weld bevel angle.
A combination of sectorial scanning with electronic scanning was used for the flat bottom hole in the bevel (simulating a lack of fusion). In this case, longitudinal ultrasound waves with half-skips are used to generate the desired angles and to ensure complete coverage of the weld. The notch in the weld toe simulates a crack next to the weld or in the Heat Affected Zone (HAZ), so a half-skip is also needed to obtain the desired coverage. In this case, transversal ultrasound waves were used, with a combination of sectorial and electronic scanning. Simulating cracks in the root, the detection of this notch was made through longitudinal waves in direct mode (no skips), as well as with a combination of electronic and sectorial scanning. Three focal laws were defined-one for each defect type. Version 6.9.25 of the Multi2000 software and MULTIX++ hardware, both from the company M2M, were used for data acquisition and processing. Table 4 presents the parameters of each focal law, as well as the corresponding beam coverage.

Scan Plan
The previously defined focal laws were calculated for a probe relative to weld positioning as shown in Figure 6, with a 2 mm offset between the wedge front face and the weld toe. This 2 mm gap exists to account for small geometric irregularities that the weld cap may exhibit. The mechanical probe movement in relation to the weld is only longitudinal-an advantage of using phased array technology. Data acquisition for each defect was made independently, with a 60 mm length scan.

Scan Plan
The previously defined focal laws were calculated for a probe relative to weld positioning as shown in Figure 6, with a 2 mm offset between the wedge front face and the weld toe. This 2 mm gap exists to account for small geometric irregularities that the weld cap may exhibit. The mechanical probe movement in relation to the weld is only longitudinal-an advantage of using phased array technology. Data acquisition for each defect was made independently, with a 60 mm length scan.

Experimental Results
When using ultrasounds for high-temperature inspections, one must account for both velocity variations and increased attenuation. A recalibration process is required to assess real velocity values. In steel, velocity changes by about 1% for each 55 °C variation in temperature [28]. In opposition, sound attenuation increases at higher temperatures. In typical fine grain carbon steel alloys, at room temperature and 5 MHz frequency, attenuation is approximately 2 dB per 100 mm one-way sound path. Due to the higher attenuation, it is often necessary to increase the instrument's gain to reach proper sensitivity [28,29]. Moreover, distance/amplitude correction (DAC) curves or TGV (Time Varied Gain) programs that are established at room temperature require adjustments. Figure 7 shows the signal amplitude variation obtained for different temperatures tested for different defects. In the results obtained, it is possible to observe that the signal amplitude decreased with increases in temperature.

Experimental Results
When using ultrasounds for high-temperature inspections, one must account for both velocity variations and increased attenuation. A recalibration process is required to assess real velocity values. In steel, velocity changes by about 1% for each 55 • C variation in temperature [28]. In opposition, sound attenuation increases at higher temperatures. In typical fine grain carbon steel alloys, at room temperature and 5 MHz frequency, attenuation is approximately 2 dB per 100 mm one-way sound path. Due to the higher attenuation, it is often necessary to increase the instrument's gain to reach proper sensitivity [28,29]. Moreover, distance/amplitude correction (DAC) curves or TGV (Time Varied Gain) programs that are established at room temperature require adjustments. Figure 7 shows the signal amplitude variation obtained for different temperatures tested for different defects. In the results obtained, it is possible to observe that the signal amplitude decreased with increases in temperature. Figure 8 shows the attenuation change with temperature for different defects. In all cases, it is possible to observe an attenuation decrease with higher temperatures. This decrease is most evident for the weld toe notch and lack of fusion defects. These results support those obtained for the maximum amplitude variation with temperature for different defects- Figure 9. As shown, as attenuation increased with higher temperatures, the signal amplitude also reduced; however, the decrease was lower for the weld root notch.
From the obtained results analysis, it is possible to verify apparent variations in the defects' dimensions along with temperature variations. Figure 10 shows the defects' apparent length variation with increases in temperature. One possible explanation is, for instance, a compromised contact between the ultrasonic transducer and the piece due to the different thermal expansion coefficients of the two materials [30,31]. For the defect weld root notch, there was an irregular variation as the temperature increased. For the weld toe notch defect, it was possible to observe some irregularity, as the size of the defect decreased as the temperature increased. However, this apparent defect dimension variation was lower for lack-of-fusion defects up to temperatures of around 200 • C. At the highest evaluated temperatures, a decrease in the value of the defect dimension was observed. The major error source was related to the ultrasonic velocity being a function of temperature, with variations in the ultrasonic wave velocity at high temperatures [30]. Measurement errors can be minimized using a moving gate control with temperature variations, normalization of the signal amplitude, automatic determination of the ultrasonic flight time, and temperature compensation.  Figure 8 shows the attenuation change with temperature for different defects. In all cases, it is possible to observe an attenuation decrease with higher temperatures. This decrease is most evident for the weld toe notch and lack of fusion defects. These results support those obtained for the maximum amplitude variation with temperature for different defects- Figure 9. As shown, as attenuation increased with higher temperatures, the signal amplitude also reduced; however, the decrease was lower for the weld root notch.    Figure 8 shows the attenuation change with temperature for different defects. cases, it is possible to observe an attenuation decrease with higher temperatures. decrease is most evident for the weld toe notch and lack of fusion defects. These re support those obtained for the maximum amplitude variation with temperatur different defects- Figure 9. As shown, as attenuation increased with higher temperat the signal amplitude also reduced; however, the decrease was lower for the weld notch.   From the obtained results analysis, it is possible to verify apparent variations in the defects' dimensions along with temperature variations. Figure 10 shows the defects' apparent length variation with increases in temperature. One possible explanation is, for instance, a compromised contact between the ultrasonic transducer and the piece due to the different thermal expansion coefficients of the two materials [30,31]. For the defect weld root notch, there was an irregular variation as the temperature increased. For the weld toe notch defect, it was possible to observe some irregularity, as the size of the defect decreased as the temperature increased. However, this apparent defect dimension variation was lower for lack-of-fusion defects up to temperatures of around 200 °C. At the highest evaluated temperatures, a decrease in the value of the defect dimension was observed. The major error source was related to the ultrasonic velocity being a function of temperature, with variations in the ultrasonic wave velocity at high temperatures [30]. Measurement errors can be minimized using a moving gate control with temperature variations, normalization of the signal amplitude, automatic determination of the ultrasonic flight time, and temperature compensation.  From the obtained results analysis, it is possible to verify apparent variations in the defects' dimensions along with temperature variations. Figure 10 shows the defects' apparent length variation with increases in temperature. One possible explanation is, for instance, a compromised contact between the ultrasonic transducer and the piece due to the different thermal expansion coefficients of the two materials [30,31]. For the defect weld root notch, there was an irregular variation as the temperature increased. For the weld toe notch defect, it was possible to observe some irregularity, as the size of the defect decreased as the temperature increased. However, this apparent defect dimension variation was lower for lack-of-fusion defects up to temperatures of around 200 °C. At the highest evaluated temperatures, a decrease in the value of the defect dimension was observed. The major error source was related to the ultrasonic velocity being a function of temperature, with variations in the ultrasonic wave velocity at high temperatures [30]. Measurement errors can be minimized using a moving gate control with temperature variations, normalization of the signal amplitude, automatic determination of the ultrasonic flight time, and temperature compensation.

Customized EC Probes
Two customized ECT probe prototypes were developed-one targeting the defects' detection on the pipe base material and the other targeting the defects' detection on the weld bead. The first developed probe comprised two rectangular planar coils operating in a bridge differential mode. The planar disposition allowed a closer contact of all the coil's windings with the material being inspected, increasing the probe's sensibility. The coils were produced on Print Circuit Board PCB technology, which enables the production of planar geometries, can be automated, is economical, and brings enhanced reproducibility. Each coil was composed by 25 turns, with a track width and spacing inbetween of 0.1 mm- Figure 11.

Customized EC Probes
Two customized ECT probe prototypes were developed-one targeting the defects' detection on the pipe base material and the other targeting the defects' detection on the weld bead. The first developed probe comprised two rectangular planar coils operating in a bridge differential mode. The planar disposition allowed a closer contact of all the coil's windings with the material being inspected, increasing the probe's sensibility. The coils were produced on Print Circuit Board PCB technology, which enables the production of planar geometries, can be automated, is economical, and brings enhanced reproducibility. Each coil was composed by 25 turns, with a track width and spacing in-between of 0.1 mm- Figure 11.

Customized EC Probes
Two customized ECT probe prototypes were developed-one targeting the defects' detection on the pipe base material and the other targeting the defects' detection on the weld bead. The first developed probe comprised two rectangular planar coils operating in a bridge differential mode. The planar disposition allowed a closer contact of all the coil's windings with the material being inspected, increasing the probe's sensibility. The coils were produced on Print Circuit Board PCB technology, which enables the production of planar geometries, can be automated, is economical, and brings enhanced reproducibility. Each coil was composed by 25 turns, with a track width and spacing inbetween of 0.1 mm- Figure 11. Figure 11. PCB probe developed for the inspection of the pipe base material. Linear excitation element cantered within the two differential coils.
Since inspections have to be performed at high temperatures over long periods of time, the selected PCB base material was a high-performance FR-4 epoxy core and prepreg laminate with a glass transition temperature (Tg) of 180 °C. However, since piping must be inspected at even higher temperatures, water cooling was applied to reduce thermal effects.
Targeting a robust, modular, and adaptable probe, a probe chassis with water cooling was developed. The chassis was composed of an insulating cup and a metallic cover. The PCB probe was fastened to an aluminum cover, where the probe connector was attached-as well as two water inlets for the refrigeration flow. For the cup, an insulating Teflon machined cup was developed. The construction process is detailed step-by-step in Figure 12, where: (a) shows the aluminum cover with the sealing O-ring and connectors for cooling and signaling; (b) and (c) the support for interconnecting the cover and the PCB; and d) the probe's overall assembly-ready insert in the insulating cup. Figure 11. PCB probe developed for the inspection of the pipe base material. Linear excitation element cantered within the two differential coils.
Since inspections have to be performed at high temperatures over long periods of time, the selected PCB base material was a high-performance FR-4 epoxy core and prepreg laminate with a glass transition temperature (Tg) of 180 • C. However, since piping must be inspected at even higher temperatures, water cooling was applied to reduce thermal effects.
Targeting a robust, modular, and adaptable probe, a probe chassis with water cooling was developed. The chassis was composed of an insulating cup and a metallic cover. The PCB probe was fastened to an aluminum cover, where the probe connector was attachedas well as two water inlets for the refrigeration flow. For the cup, an insulating Teflon machined cup was developed. The construction process is detailed step-by-step in Figure 12, where: (a) shows the aluminum cover with the sealing O-ring and connectors for cooling and signaling; (b) and (c) the support for interconnecting the cover and the PCB; and d) the probe's overall assembly-ready insert in the insulating cup. The second probe targeted the detection of weld bead defects and was also composed of two coils in bridge-differential mode. The probe was designed so that the coils remained in the same position along the bead and maintained a similar influence over the weald bead on the two coils' signals. This property allows for the reduction of the probe response to weld bead profile variations that otherwise mask the typically small response to lowest-dimension defects. As the defect orientation is naturally unknown, the probe must be also sensitive to defects with any alignment with respect to the weld bead. The adopted solution was the orthogonal crossing coils shown in Figure 13, which are often employed in the inspection of other welded parts.
A similar construction strategy as the one in the first probe was adopted. Figure 13 shows the developed chassis in each assembly step: (a) shows the overall probe assembly The second probe targeted the detection of weld bead defects and was also composed of two coils in bridge-differential mode. The probe was designed so that the coils remained in the same position along the bead and maintained a similar influence over the weald bead on the two coils' signals. This property allows for the reduction of the probe response to weld bead profile variations that otherwise mask the typically small response to lowestdimension defects. As the defect orientation is naturally unknown, the probe must be also sensitive to defects with any alignment with respect to the weld bead. The adopted solution was the orthogonal crossing coils shown in Figure 13, which are often employed in the inspection of other welded parts. must be also sensitive to defects with any alignment with respect to the weld bead. The adopted solution was the orthogonal crossing coils shown in Figure 13, which are often employed in the inspection of other welded parts.
A similar construction strategy as the one in the first probe was adopted. Figure 13 shows the developed chassis in each assembly step: (a) shows the overall probe assembly cut-out; (b) the lid with the sealing O-ring and connectors for cooling and signaling; (c) the FDM-printed support used to hold the orthogonal coils, and (d) the final external aspect. The external shape of the cup can also be seen in Figure 13, which was specially developed to produce the correct positioning of the probe before the welding.

Experimental Results
The customized Eddy current probes were experimentally validated using the automated inspection system presented in Section 2.2, Figure 2a.

Base Material Inspection
For the experimental validation of the base material probe in Figure 12, three rectangular defects were artificially produced, being 0.5 mm wide, 0.4 mm deep and 10 A similar construction strategy as the one in the first probe was adopted. Figure 13 shows the developed chassis in each assembly step: (a) shows the overall probe assembly cut-out; (b) the lid with the sealing O-ring and connectors for cooling and signaling; (c) the FDM-printed support used to hold the orthogonal coils, and (d) the final external aspect. The external shape of the cup can also be seen in Figure 13, which was specially developed to produce the correct positioning of the probe before the welding.

Experimental Results
The customized Eddy current probes were experimentally validated using the automated inspection system presented in Section 2.2, Figure 2a.

Base Material Inspection
For the experimental validation of the base material probe in Figure 12, three rectangular defects were artificially produced, being 0.5 mm wide, 0.4 mm deep and 10 mm high and with an angle of 0 • , 45 • and 90 • in a 329 mm diameter 16Mo3 steel pipe. The gathered results shown in Figure 14 were obtained at 1 MHz frequency while the probe travelled in the X direction, centered with the defect. Through the superposition of the signals, the characterization of the defects did not suffer from temperature increases, which indicates that the probe cooling was effective.
One-dimensional scans are useful for studying probe signal characteristics; however, C-scans are required to cover the whole area of the inspected pipe. Figure 15 shows the output signal in a C-scan performed over a 200 mm × 30 mm area containing the same defects. All three defects were clearly detected in the C-scan, which additionally provided some insight into the defects' morphologies, orientations, and dimensions.

Weld Bead Inspection
Inspections were carried out on the two artificially manufactured defects on the outer surface of the tube. Scans along the perimeter of the tube were carried out on both the right and left sides of the weld bead, Figure 16. Measurements were recorded continuously while the automated inspection system was moving along the pipe perimeter. The excitation frequency used was 300 kHz in all tests. mm high and with an angle of 0°, 45° and 90° in a 329 mm diameter 16Mo3 steel pipe. The gathered results shown in Figure 14 were obtained at 1 MHz frequency while the probe travelled in the X direction, centered with the defect. Through the superposition of the signals, the characterization of the defects did not suffer from temperature increases, which indicates that the probe cooling was effective. One-dimensional scans are useful for studying probe signal characteristics; however, C-scans are required to cover the whole area of the inspected pipe. Figure 15 shows the output signal in a C-scan performed over a 200 mm × 30 mm area containing the same defects. All three defects were clearly detected in the C-scan, which additionally provided some insight into the defects' morphologies, orientations, and dimensions.

Weld Bead Inspection
Inspections were carried out on the two artificially manufactured defects on the outer surface of the tube. Scans along the perimeter of the tube were carried out on both the right and left sides of the weld bead, Figure 16. Measurements were recorded continuously while the automated inspection system was moving along the pipe perimeter. The excitation frequency used was 300 kHz in all tests.  Figure 17 shows the defects present in the weld beads-approximately 8 mm long, 1 mm wide, and 3 mm deep. One centered with the weld bead and one was at the weld bead's border with the base material. Besides the background signal resulting from the weld bead surface profile variations, a signal peak caused by the defects' presence stood out.

Weld Bead Inspection
Inspections were carried out on the two artificially manufactured defects on the outer surface of the tube. Scans along the perimeter of the tube were carried out on both the right and left sides of the weld bead, Figure 16. Measurements were recorded continuously while the automated inspection system was moving along the pipe perimeter. The excitation frequency used was 300 kHz in all tests. Figure 16. ECT probe developed for the weld bead inspection performing a scan on the bead's right side. Figure 17 shows the defects present in the weld beads-approximately 8 mm long, 1 mm wide, and 3 mm deep. One centered with the weld bead and one was at the weld bead's border with the base material. Besides the background signal resulting from the weld bead surface profile variations, a signal peak caused by the defects' presence stood out.

Conclusions
This work demonstrates the application of UT and EC for high-temperature inservice industrial components. Although the target application related to the paper industry, benefits could materialize across a wide range of industries including chemical and energy production. The ability to perform inspections while continuously operating reduces the frequency of planned outages. On the other hand, the possibility of monitoring known defects and degradation allows for the taking of informed decisions on whether or not interrupt operations and to better plan future interventions.
The UT probes' designs for active cooling proved to be effective and favourable for good ultrasound propagation at the same time. The wedge also provided some thermal insulation, helping to keep the probe under operating conditions. The reported results showed the adopted solutions' effectiveness up to 200 °C and that temperature effects can be compensated for by a moving gate control with temperature variation, normalization of the signal amplitude, automatic determination of the ultrasonic flight time, and temperature compensation.
Despite the high lift-off required for the high-temperature EC testing, both differential probes obtained very good results. The PCB probe showed improved results with a higher signal-to-noise ratio, and high temperatures did not have a significant impact due the effective cooling of the ECT probes. The produced prototypes allowed experimental validation, with results demonstrating almost no influence when

Conclusions
This work demonstrates the application of UT and EC for high-temperature in-service industrial components. Although the target application related to the paper industry, benefits could materialize across a wide range of industries including chemical and energy production. The ability to perform inspections while continuously operating reduces the frequency of planned outages. On the other hand, the possibility of monitoring known defects and degradation allows for the taking of informed decisions on whether or not interrupt operations and to better plan future interventions.
The UT probes' designs for active cooling proved to be effective and favourable for good ultrasound propagation at the same time. The wedge also provided some thermal insulation, helping to keep the probe under operating conditions. The reported results showed the adopted solutions' effectiveness up to 200 • C and that temperature effects can be compensated for by a moving gate control with temperature variation, normalization of the signal amplitude, automatic determination of the ultrasonic flight time, and temperature compensation.
Despite the high lift-off required for the high-temperature EC testing, both differential probes obtained very good results. The PCB probe showed improved results with a higher signal-to-noise ratio, and high temperatures did not have a significant impact due the effective cooling of the ECT probes. The produced prototypes allowed experimental validation, with results demonstrating almost no influence when temperatures were raised up to 300 • C.